PROJECT Ι. 2 MICRO AND NANOFABRICATION USING LITHOGRAPHY ...imel. · PDF filePROJECT...
Embed Size (px)
Transcript of PROJECT Ι. 2 MICRO AND NANOFABRICATION USING LITHOGRAPHY ...imel. · PDF filePROJECT...
24 INSTITUTE OF MICROELECTRONICS (IMEL) NCSR DEMOKRITOS - Project I
PROJECT . 2 MICRO AND NANOFABRICATION USING LITHOGRAPHY AND PLASMA ETCHING
Key researchers: E. Gogolides, A. Tserepi
Permanent Researcher: V. Constantoudis
Researchers on Contract: G. Kokkoris
Post Doctoral fellows: A. K. Gnanappa, D. Moschou, N. Vourdas, K. Tsougeni, G. Papadakis
Collaborating researchers: S. Chatzandroulis, K. Misiakos, I. Raptis, P. Argitis, P. Normand, P. Dimitrakis
PhD candidates: M.- E. Vlachopoulou, A. Malainou, D. Kontziampasis, K. Ellinas, G. Aksenov, V.K. Murugesan Kuppuswamy, N. Skoro, A. Smyrnakis
MSc Students: A. Zeniou, I. Kouris, E. Mavraki, D. Zervas, N. Karasmani, M. Kalimeri
External collaborators: S.Kakabakos, P.Petrou (IRRP, NCSR-D), S.Garbis, A.Vlahou, P.Zerefos, S.Pagakis (IIBEAA, Greece), G.Kaltsas (TEI of Athens, Greece), A.Boudouvis, A.Papathanasiou, D.P.Papageorgiou, N.Cheimarios (NTUA, Greece), E.Sarantopoulou (NHRF, Greece), E.Gizeli (FORTH Greece), K.Beltsios, I.Panagiotopoulos (U. Ioannina, Greece), C.Cardinaud (U. Nantes, France), G.Gallatin (NIST, USA), A.Speliotis (IMS, NCSR-D), R.Gronheid, A.P.Vaglio (IMEC), W.Coene, M.Riepen, M.Van Kampen (ASML), D.Ehm (Zeiss), T.Rudin, S.E.Pratsinis (ETH Zurich), G.L.Vignoles (U. BordeauxI), Ph.Supiot (U. of Lille I)
SPAM, Marie Curie-ITN, Contract No 215723 Lab-on-chip Corralia-GSRT Contract No 2--/- DNA on waves: an integrated diagnostic system GSRT Contract No LS7(276)
Our objective is to use our rich plasma nanoscience and nanoassembly toolbox as an enabling technology for a variety of applications including Surface Science, Life Sciences and Energy, as well as for fundamental studies in these fields. More specifically, we use various top down and bottom up patterning processes followed by plasma etching / processing not only for nano-electronics and MEMs, but also for surface wetting control, surface engineering, microfluidics, microarrays, lab-on-a-chip fabrication, and Nanowire Fabrication for Energy:
For nano-electronics, we focused on simulation of Line Edge Roughness (LER) transfer during plasma etching and the formation of Contact Edge Roughness (CER). Also, we generated synthesized SEM images to study noise effects and applied the developed software in EUV lithography. (see section A)
For Life Science applications, Plasma Processing was used to fabricate microfluidics, lab on a chip, and microarrays. Several analytical microfluidic devices were developed: (a) An affinity chromatography chip for phosphopeptide enrichment with capacity comparable to commercial off-line TiO2 tips, using a cost-effect flame pyrolysis method on thermosensitive polymeric substrates. (b) A chip for DNA amplification using continuous flow PCR. (c) A microfluidic device with controlled wetting properties and controlled protein adsorption on rough walls. In addition we demonstrated DNA microarrays on plasma nanotextured Polystyrene slides applied for improved detection of gene mutations, as well as protein microarrays with improved sensitivity and uniformity on photolithographed and plasma modified glass substrates (see section B)
Plasma Nanoassembly or colloidal particle self-assembly was used to create nanopillars on Silicon, leading to extremely low Si reflectance. We demonstrated cryogenic etching processes of Silicon leading to nanoscale Silicon pillars of high aspect ratio (>20:1). Plasma nanotextured surfaces coated with plasma deposited Teflon films led to superamphiphobic (water and oil resistant) surfaces. The mechanical and thermodynamic stability of these surfaces was examined using drop pressing experiments. Finally we have continued the work of plasma directed organization and shown the effects of polymeric material and etching time on the self-organization of these nanodots (see section C)
Simulation work on plasma etching, plasma deposition, CVD and plasma nanoscience assists process design and understanding and is described in section D.
Work on the characterization and modeling of micro- and nanofabricated structures has also been initiated (see section E)
25 INSTITUTE OF MICROELECTRONICS (IMEL) NCSR DEMOKRITOS - Project I
RESEARCH RESULTS IN 2011 A. Micro and Nano Lithography: Simulation and Metrology
This year, the work of our group in this area was focused on the issue of sidewall roughness of lithographic features, which becomes increasingly important in the semiconductor industry as the size of printed features is shrinking to sub-30nm scale. It is believed that the sidewall roughness of lines and contacts and the related variability would be one of the main obstacles to be overcome in near future lithographies. The results of our research concern both simualtion and metrology issues with emphasis on LER transfer during etching, Contact Edge Roughness simulation and metrology and SEM image noise effects on CER measurement.
A1 Line Edge Rougness (LER) transfer during plasma etching
G. Kokkoris, V. Constantoudis, E. Gogolides
The line edge roughness transfer from the resist to the underlying substrate via plasma etching is studied with a 3d modeling framework. The framework includes the generation of 3d rough resist lines with predetermined roughness parameters [root mean square roughness (), correlation length (), and roughness exponent]. The pattern transfer of the generated 3d lines to the substrate is captured by an abstractive geometric model: Plasma etching is considered anisotropic and the shadowing of the incident ions by the protrusions of the initial resist sidewall determines the roughness of the substrate sidewall. Shadowing is enough to induce the striations and the reduction of at the substrate sidewall. The effect of the sidewall roughness ( and ) and shape (thickness and sidewall slope) of the initial resist line as well as the etching selectivity and etching depth on a) and b) the slope of the substrate sidewall is investigated. A linear relation between of the substrate and of the initial resist sidewalls is found, consistently with pertinent experimental studies. It is found that the reduction of is favored by a low correlation length of the initial resist sidewall and by thicker resist films. The decrease of of the initial resist sidewall, the increase of the etching selectivity, and the increase of the initial resist thickness favors a slope of the substrate sidewall closer to 90
o. The slope of the initial resist sidewall affects
the slope of the substrate sidewall only for low values of .
Production of 3d rough line
(plasma etching )
Fig.1. (a) A plane rough surface with specific roughness parameters ( = 2, = 20, roughness exponent = 0.4). (b) A 3d smooth line. (c) A 3d rough line coming from the superimposition of the plane rough surface (Fig. 1a) onto the smooth 3d line (Fig. 1b). (d) The 3d line of the substrate after plasma etching and removal of resist. Notice the formation of striations at the sidewall of the substrate. The etching depth is 150 and the etching selectivity of the substrate over the resist is 3.
26 INSTITUTE OF MICROELECTRONICS (IMEL) NCSR DEMOKRITOS - Project I
A2 Modeling of Contact Edge Roughness and Critical Dimension Uniformity (CDU) formation
V.-K. Murugesan Kuppuswamy, V. Constantoudis
Several modeling and simulation studies have been devoted to Line Edge Roughness (LER) formation in the present and near future lithographies and especially, in Extreme Ultra-Violet Lithography (EUVL) which is the stronger candidate to replace 193nm immersion lithography in the manufacturing of Integrated Circuits (see for example the stochastic simulation for LER developed in our group and presented in previous year reports). Recently. however, the roughness of contact holes (contact hole or edge Roughness, CHR/CER) and mainly their dimensional variability (usually described as critical dimension uniformity, CDU) has also attracted a lot of interest in EUVL community, due to the difficulty in reducing these to the allowable limits. In order to reach these limits, we can use the experience gained in LER reduction studies. However, it is not clear at which level CER behaves in a similar way to LER, given the different topology of contacts compared to lines (circular vs. linear). Thus, a question that can be asked is to explore the implications of this difference in the process effects on CER with respect to LER. In order to investigate this issue, we developed a numerical model for CER inspired by the analytical modeling for LER proposed by Gallatin [Proc. of SPIE 2005 p.38]. This simplified simulation modeling of the lithographic process with code name CERSIM takes into account the discrete effects of photons (shot noise), the acid diffusion and a simplified version of critical ionization model for dissolution. Its successive steps are shown in Fig. 2.
Fig.2. Steps of the simplified simulation of lithographic process for CER formation with emphasis on shot noise and acid diffusion effects.
The first application of the modeling will be to study the effects of exposure dose on CER
and CDU. According to very recent experimental findings, the RMS of CER increases at high doses contrary to LER behavior and shot noise expectation